Banishing Bottom Blisters
If your classic-plastic cruiser contracts the pox, take these steps to ensure years more of trouble-free service. "Projects" from our April 2012 issue.
The Mason’s hull, either by luck or due to sitting on the hard for several months, was dry. Before we rolled on multiple layers of epoxy barrier coating—which should protect the laminate from water for years—it was a good time to remove the gelcoat and find out what we really had on our hands. A guy with a peeling machine shaved the old gelcoat from the keel to the waterline. Now completely “bare,” the hull showed extensive areas of dry, unsaturated mat strands, and the peeling operation left slight furrows. The boat’s hull under the waterline needed some fairing.
To protect myself from fiberglass particles, I zipped on a white Tyvek suit, put on a respirator and ear protectors, and went at it. Here I made the mistake of grinding with 5-inch discs of 36-grit sandpaper. I should’ve used a grinder capable of carrying 8-inch discs sitting on a soft pad. Better yet, I should’ve hired someone to do it. I did remove all the dry fibers but, due to the small disc, the surface still needed fairing. I troweled on epoxy resin thickened with colloidal silica, both WEST System products. This had to be sanded before rolling on coats of Interlux’s InterProtect 2000, an epoxy-based barrier product. First, I washed the surface with water and light detergent in order to remove the amine blush, a waxy film produced by curing epoxy. A 44-foot boat with a long keel, a 32-foot waterline, and a nearly 7-foot draft towered over Nancy and me like a cliff of cured epoxy as hard as granite. The task of fairing it all with orbital high-speed sanders, followed by wet sanding, took us three long days.
Rolling on the InterProtect 2000 doesn’t require sanding in between; we easily put two coats on in a day. However, the stuff contains some strong, nasty solvents, so we wore respirators and gloves. I followed the sixth coat with two rounds of antifouling paint. All that was left to do was to move the jack stands and block the boat higher to address the untreated spots.
The project, carried out in the Florida summer heat, took some stamina. I also added a bit of extra work for my own piece of mind and satisfaction. Many fiberglass boats, including ours, were built in split molds. After the hull was laminated, the mold had been opened sideways, leaving a visible seam that ran from the stem along the bottom of the keel and up to the sternpost. The builders had filled it with cheap polyester putty and sprayed it with gelcoat. Though it shouldn’t affect the strength of the hull, in our case the peeling process opened up this seam; with all the crumbling putty, it looked awful.
To rectify it, I removed the loose putty first and filled the gaps with thickened epoxy resin. Next, I covered the seam with a layer of biaxial cloth and epoxy resin right along the boat’s backbone, from the stem over the keel to the stern. It took a few more days of extra fairing and sanding, but it made me much happier, especially when I recalled past collisions with tree trunks at sea.
Removing a certain amount of the deteriorated laminate may seem worrisome. However, remember that the gelcoat and the resin-starved mat didn’t contribute anything to the strength of the hull. Early glass boats often had extremely thick hulls, and stripping the outer layers won’t affect the strength. Just because it was built a long time ago by a reputable builder doesn’t guarantee a good laminate job. It basically comes down to this: Who was the foreman of the glass shop? Should you need to dig deeper than the gelcoat and mat to reach the solid laminate, seek professional advice from a truly experienced surveyor or a respected boatyard foreman. Some beautiful yachts with great sailing qualities have had to be reglassed totally within 10 years of launching by owners dedicated to the design. On the other hand, many hulls never contract blisters after decades afloat. If yours isn’t one of those, this project to eradicate hull blisters should keep a yacht going strong for many decades.
Longtime Cruising World contributors Tom and Nancy Zydler have refit their Mason 44, Frances B, for extensive high-latitude voyaging.